Multifunctional nanocomposite hollow fiber membranes by ... - STrIPS- Multifunctional
Embed Size (px)
Transcript of Multifunctional nanocomposite hollow fiber membranes by ... - STrIPS- Multifunctional
Multifunctional nanocomposite hollow fibermembranes by solvent transfer induced phaseseparationMartin F. Haase1, Harim Jeon2,3, Noah Hough1, Jong Hak Kim 3, Kathleen J. Stebe2 & Daeyeon Lee2
The decoration of porous membranes with a dense layer of nanoparticles imparts useful
functionality and can enhance membrane separation and anti-fouling properties. However,
manufacturing of nanoparticle-coated membranes requires multiple steps and tedious pro-
cessing. Here, we introduce a facile single-step method in which bicontinuous interfacially
jammed emulsions are used to form nanoparticle-functionalized hollow fiber membranes. The
resulting nanocomposite membranes prepared via solvent transfer-induced phase separation
and photopolymerization have exceptionally high nanoparticle loadings (up to 50 wt% silica
nanoparticles) and feature densely packed nanoparticles uniformly distributed over the entire
membrane surfaces. These structurally well-defined, asymmetric membranes facilitate con-
trol over membrane flux and selectivity, enable the formation of stimuli responsive hydrogel
nanocomposite membranes, and can be easily modified to introduce antifouling features. This
approach forms a foundation for the formation of advanced nanocomposite membranes
comprising diverse building blocks with potential applications in water treatment, industrial
separations and as catalytic membrane reactors.
DOI: 10.1038/s41467-017-01409-3 OPEN
1 Rowan University, Henry M. Rowan College of Engineering, Glassboro, NJ 08028, USA. 2Department of Chemical and Biomolecular Engineering, Universityof Pennsylvania, Philadelphia, PA 19104, USA. 3 Department of Chemical and Biomolecular Engineering, Yonsei University, Seoul, 03722, South Korea.Correspondence and requests for materials should be addressed to M.F.H. (email: firstname.lastname@example.org) or to K.J.S. (email: email@example.com)or to D.L. (email: firstname.lastname@example.org)
NATURE COMMUNICATIONS |8: 1234 |DOI: 10.1038/s41467-017-01409-3 |www.nature.com/naturecommunications 1
Membrane separations are promising alternatives tothermal separations because of their high-energy effi-ciency, their applicability to mixtures containing ther-mally sensitive materials, and their scalability1. For example,water treatment membranes are currently widely used in large-scale reverse osmosis desalination plants and in small-scale per-sonalized ultrafiltration membrane cartridges. Solar poweredsmall-scale ultrafiltration membrane systems are cur-rently employed in remote areas with limited access to safedrinking water or in times of natural disasters and emergencies.Key considerations in the development of new membranesinclude cost and scalability, high chemical/thermal stability, highselectivity, and high permeability2. Membranes should also bedesigned to separate multicomponent mixtures, be resistant tofouling, and have excellent mechanical and chemical stability3.
Nanocomposite membranes composed of mixtures of nano-particles and polymers have many of these attributes, makingthem attractive for a variety of applications. Their hydrophilicity4,porosity5, charge density6, thermal and mechanical stability7, 8
can be tailored by locating nanoparticles with specific propertiesand functionality on the surface or within the matrix of thepolymer scaffold. In particular, nanocomposite membranes withsurface-located nanoparticles can provide unique features such asantibacterial9, photocatalytic10, or adsorptive11 capabilities. Forinstance, microporous zeolites12 have been shown to enhancemembrane fluxes at high selectivity for molecular separations13.Silver14 or copper15 nanoparticles also have been demonstrated tointroduce antimicrobial functionalities. The photocatalytic activ-ity of surface located titanium dioxide nanoparticles has beenshown to introduce self-cleaning properties16.
Despite these advantages, nanoparticle-laden polymer mem-brane fabrication presents major processing challenges, limitingtheir widespread utilization. Such membranes are typically fabri-cated by incorporation of nanoparticles directly into the polymersolutions for membrane formation or by modification of
preformed polymer membranes with nanoparticles17. The formerapproach is challenging due to unfavorable interactions betweenthe polymers and nanoparticles that drive nanoparticle aggrega-tion. Thus, nanoparticles, introduced to concentrated polymersolutions used for immersion precipitation, tend to distribute non-uniformly on the membrane surface, compromising the mem-brane structure and properties1821. The latter approach circum-vents this nanoparticle aggregation issue, however, modification ofpre-formed membranes typically requires multistep processes thatexploit specific nanoparticle-/membrane-binding mechanisms22.Furthermore, nanoparticles may only coat the very outermostsurface of the membrane23. Finally, weakly surface-adherednanoparticles can detach from the membrane during usage andrelatively low nanoparticle loading is typically achieved4, 24, 25.
Here, we introduce an approach for the fabrication of nano-composite membranes with nanoparticles densely and uniformlydistributed over the entire surface of the porous membrane. Ourapproach facilitates previously unattainable nanoparticle loadingsand placement on membranes and enables the single step fabri-cation of nanocomposite membranes composed of highly cross-linked polymers (here polyacrylates) with pronounced chemicalresistance. This ability to manufacture a highly cross-linkednanocomposite membrane has unique advantages; such a mem-brane cannot be easily formed via traditional immersion pre-cipitation approaches without specifically functionalizedpolymers that allow for post-processing26.
The highly cross-linked nanocomposite membranes introducedin this work are produced by the combination of recentlydiscovered bicontinuous interfacially jammed emulsion gels(bijels)2730 and some aspects of the classical membrane fabri-cation techniques known as non-solvent-induced phase separa-tion (NIPS) or immersion precipitation3133. Recently, we havedeveloped solvent transfer-induced phase separation (STRIPS)34,35 to enable continuous manufacturing of STRIPS bijel fibers.Unlike NIPS, STRIPS does not employ polymers, but rather uses
Ternarymixture A +
Particles +CTAB + initiator
Silica + CTAB
EthanolEthanol transtransfererEthanol transfer
Rapid demixingRapid demixing on surfaceon surfaceRapid demixing on surface
DelayedDelayed demixingdemixingDelayed demixing
Fig. 1 Formation of hollow fiber membranes by STRIPS. a Schematics of hollow fiber membrane formation. The co-extrusion of a silica nanoparticle dopedmonomer solution (ternary fluid) and water (bore fluid and sweeping fluid) yields a hollow fiber. To produce a uniform hollow core, the bore-fluid nozzlemust be centered, (as is assured by a square capillary that serves to fix its location, see Supplementary Methods), and the bore fluid viscosity must beadjusted by addition of high molecular mass polyethylene glycol (1 wt% PEG, 600 kDa). Rapid solvent transfer to the outer water phase and to the borefluid induces phase separation on the fiber surfaces. Delayed solvent transfer in the radial direction generates aligned internal macrovoids. Interfacialnanoparticle jamming yields a nanoparticle-stabilized bicontinuous liquid monomer/water scaffold on the fiber surface. The monomers are polymerized byUV-light irradiation, resulting in a hollow, porous polymer/nanoparticle composite fiber. b Aligned fibers are collected in a rotating glass cylinder filled withwater. Fiber exiting the orifice is guided to horizontal orientation by the curved outer channel. Prior to polymerization, the hollow nanoparticle-stabilizedliquid fibers are fragile (tensile strength ranging from 0.6 to 4 kPa)35; flow- and collection bath rotation must be delicately controlled to prevent fractureand defect formation (see Supplementary Methods, Supplementary Note 6). However, upon polymerization, the hollow fiber membrane can be washedand dried without compromising structural integrity. c Photograph of dried hollow fiber membrane, scale bar 0.5 cm. d SEM micrographs reveal the internal(scale bar 200 m, inset 20 m) and surface structures (scale bar 5 m) of fibers fabricated with ternary flow rate QT= 10ml hl and bore fluid flow rateQB= 15 ml h1 at constant water flow rate of 1 ml min1
ARTICLE NATURE COMMUNICATIONS | DOI: 10.1038/s41467-017-01409-3
2 NATURE COMMUNICATIONS |8: 1234 |DOI: 10.1038/s41467-017-01409-3 |www.nature.com/naturecommunications
liquid monomers for membrane formation. Asymmetric mem-branes are obtained by arresting the phase separation of themonomers and water with silica nanoparticles that form densejammed layers at the oil-water interface; the monomers are the